DOI: 10.17188/1475837
title: Materials Data on Sr6Ca2MnFe7O20 by Materials Project

description: Sr6Ca2MnFe7O20 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are twenty-four inequivalent Sr2+ sites. In the first Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.50–3.18 Å. In the second Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.46–3.16 Å. In the third Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.48–2.97 Å. In the fourth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.50–2.81 Å. In the fifth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.47–2.97 Å. In the sixth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.47–2.89 Å. In the seventh Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.50–2.92 Å. In the eighth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.50–2.92 Å. In the ninth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.46–3.18 Å. In the tenth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.47–2.95 Å. In the eleventh Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.47–2.99 Å. In the twelfth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.43–2.99 Å. In the thirteenth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.49–3.17 Å. In the fourteenth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.51–2.82 Å. In the fifteenth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.46–3.17 Å. In the sixteenth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.43–3.04 Å. In the seventeenth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.49–2.94 Å. In the eighteenth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.54–2.89 Å. In the nineteenth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.50–2.96 Å. In the twentieth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.52–2.92 Å. In the twenty-first Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.44–3.19 Å. In the twenty-second Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.52–2.93 Å. In the twenty-third Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.46–2.98 Å. In the twenty-fourth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.53–2.89 Å. There are eight inequivalent Ca2+ sites. In the first Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to seven O2- atoms. There are a spread of Ca–O bond distances ranging from 2.34–2.60 Å. In the second Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to seven O2- atoms. There are a spread of Ca–O bond distances ranging from 2.34–2.62 Å. In the third Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to seven O2- atoms. There are a spread of Ca–O bond distances ranging from 2.34–2.63 Å. In the fourth Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to seven O2- atoms. There are a spread of Ca–O bond distances ranging from 2.35–2.62 Å. In the fifth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.36–2.91 Å. In the sixth Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.35–2.98 Å. In the seventh Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.34–3.01 Å. In the eighth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.34–2.88 Å. There are four inequivalent Mn3+ sites. In the first Mn3+ site, Mn3+ is bonded to four O2- atoms to form MnO4 tetrahedra that share corners with two FeO6 octahedra, a cornercorner with one MnO4 tetrahedra, and a cornercorner with one FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 21–29°. There are a spread of Mn–O bond distances ranging from 1.91–2.06 Å. In the second Mn3+ site, Mn3+ is bonded to four O2- atoms to form MnO4 tetrahedra that share corners with two FeO6 octahedra, a cornercorner with one MnO4 tetrahedra, and a cornercorner with one FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 22–24°. There are a spread of Mn–O bond distances ranging from 1.90–2.00 Å. In the third Mn3+ site, Mn3+ is bonded to four O2- atoms to form MnO4 tetrahedra that share corners with two FeO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 24–25°. There are a spread of Mn–O bond distances ranging from 1.93–2.03 Å. In the fourth Mn3+ site, Mn3+ is bonded to four O2- atoms to form MnO4 tetrahedra that share corners with two FeO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 22–25°. There are a spread of Mn–O bond distances ranging from 1.88–2.03 Å. There are twenty-eight inequivalent Fe3+ sites. In the first Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with four FeO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 10–14°. There are a spread of Fe–O bond distances ranging from 1.99–2.27 Å. In the second Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with four FeO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 7–8°. There are a spread of Fe–O bond distances ranging from 1.99–2.27 Å. In the third Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with four FeO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 10–11°. There are a spread of Fe–O bond distances ranging from 1.98–2.22 Å. In the fourth Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with four FeO6 octahedra, a cornercorner with one MnO4 tetrahedra, and a cornercorner with one FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 4–9°. There are a spread of Fe–O bond distances ranging from 2.00–2.26 Å. In the fifth Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with four FeO6 octahedra, a cornercorner with one MnO4 tetrahedra, and a cornercorner with one FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 9–10°. There are a spread of Fe–O bond distances ranging from 1.99–2.16 Å. In the sixth Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with four FeO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 7–8°. There are a spread of Fe–O bond distances ranging from 1.99–2.23 Å. In the seventh Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with four FeO6 octahedra, a cornercorner with one MnO4 tetrahedra, and a cornercorner with one FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 8–13°. There are a spread of Fe–O bond distances ranging from 2.00–2.15 Å. In the eighth Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with four FeO6 octahedra, a cornercorner with one MnO4 tetrahedra, and a cornercorner with one FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 4–8°. There are a spread of Fe–O bond distances ranging from 2.00–2.23 Å. In the ninth Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with four FeO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 10–14°. There are a spread of Fe–O bond distances ranging from 2.00–2.27 Å. In the tenth Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with four FeO6 octahedra, a cornercorner with one MnO4 tetrahedra, and a cornercorner with one FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 4–8°. There are a spread of Fe–O bond distances ranging from 2.00–2.28 Å. In the eleventh Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with four FeO6 octahedra, a cornercorner with one MnO4 tetrahedra, and a cornercorner with one FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 8–11°. There are a spread of Fe–O bond distances ranging from 1.98–2.19 Å. In the twelfth Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with four FeO6 octahedra, a cornercorner with one MnO4 tetrahedra, and a cornercorner with one FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 7–8°. There are a spread of Fe–O bond distances ranging from 2.00–2.21 Å. In the thirteenth Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with four FeO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 9–11°. There are a spread of Fe–O bond distances ranging from 1.97–2.26 Å. In the fourteenth Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with four FeO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 5–7°. There are a spread of Fe–O bond distances ranging from 1.99–2.23 Å. In the fifteenth Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with four FeO6 octahedra, a cornercorner with one MnO4 tetrahedra, and a cornercorner with one FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 8–10°. There are a spread of Fe–O bond distances ranging from 2.00–2.19 Å. In the sixteenth Fe3+ site, Fe3+ is bonded to six O2- atoms to form FeO6 octahedra that share corners with four FeO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 7–9°. There are a spread of Fe–O bond distances ranging from 1.99–2.24 Å. In the seventeenth Fe3+ site, Fe3+ is bonded to four O2- atoms to form FeO4 tetrahedra that share corners with two FeO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 30–40°. There are a spread of Fe–O bond distances ranging from 1.88–1.96 Å. In the eighteenth Fe3+ site, Fe3+ is bonded to four O2- atoms to form FeO4 tetrahedra that share corners with two FeO6 octa